Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA


 Domenic Watkins
 1 years ago
 Views:
Transcription
1 Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics materials are widely used in the automotive industry with the injection molding process. For structural applications, the most common reinforcement is to add discontinuous short glass fibers to increase the stiffness and the mechanical properties. Due to the aspect ratio of the fibers and the fiber orientation inside the material, the mechanical properties of the reinforced polymer will become anisotropic. The injection molding process will orient the fibers regarding the material flow inside the mold during the filling phase. With injection molding simulation tools, the fiber orientation is one of the key outputs that can be used for the structural product simulation. Faurecia has developed a mapping tool to transfer mold filling fiber orientation results into LSDyna structural mesh for the product simulation. Each elements, each integration points over the thickness is oriented according fiber directions of the mold filling simulation results and some specific anisotropic linear elastic / nonlinear viscoplastic mechanical properties are affected according fiber orientation tensors results. Anisotropic characterization of the composite material associated with composite homogenization simulations is used to fill the different mechanical properties of the fiber orientation discretization. The fiber reinforced thermoplastic is discretized into several *MAT_ANISOTROPIC_ELASTIC_PLASTIC regarding different fiber orientation tensors possibilities, from a diffuse isotropic fiber orientation to a highly orthotropic fiber orientation. Failure criteria are integrated with the *MAT_ADD_EROSION features with the same fiber orientation tensor discretization as for the *MAT_ANISOTROPIC_ELASTIC_PLASTIC. The use of maximum stress and strain versus strain rate and triaxiality is used to modelize rupture under crash solicitations and fiber orientation. Validations and correlations have been performed on a PA6 I GF35 reference beam under static and dynamic three points bending. 2 Rheology simulation and fiber orientation mapping process The mold filling simulation will predict the material flow inside the mold regarding material viscosity, temperature, pressure, and shear rate. The fibers are aligned according to the flow orientation. The simulation is using FolgarTucker equation to estimate fiber orientation regarding material flow. One of the key outputs for this process simulation will be the fiber orientation for each element, each integration point over the thickness (12 layers over thickness in general). The fiber orientation is written in an ascii file in a tensor format.
2 The fiber orientation results are visualized with sized colored vectors indicating the three principal directions of the fibers. The biggest vector is the major principal direction with an associated color which is indicating the ratio of fibers oriented in the major principal fiber direction. The second and third principal fiber directions are orthogonal to the first direction with specific fiber ratio for each. Fig.1: Principal fiber orientation with fibers highly oriented in the major direction (left) and with mixed orientations between the two principal s directions (right) Faurecia has developed a mapping tool that will orient every element and every thickness integration point of the LSDyna structural mesh regarding the major principal fiber direction. Some specific *MAT_ANISOTROPIC_ELASTIC_PLASTIC anisotropic nonlinear elastoviscoplastic material models are affected for each integration point over the thickness regarding the fiber ratio between the principals fibers directions. The material is oriented according the major principal fiber direction with aopt=0 (material axis oriented according element nodes) with a *PART_COMPOSITE for each element indicating the material ID per layer, the layer thickness, and the layer orientation according to the major fiber direction. See example below for one element: *PART_COMPOSITE POUTRE_PLASTIQUE_1_030209_TOP_RO_RIB_2.4_PROP1000 $# pid elform shrf nloc marea hgid adpopt ithelfrm $# mid1 thick1 b1 ithid1 mid2 thick2 b2 ithid *ELEMENT_SHELL_BETA $# eid pid n1 n2 n3 n4 n5 n6 n7 n $# thic1 thic2 thic3 thic4 psi Composite homogenization and material orientation discretization A specific anisotropic material characterization is required with coupons cut into one side injection gate plates. The coupons are cut with 0, 45, and 90 angles versus material flow. The fiber orientation inside the plate is measured by tomography to know exactly the microstructure fiber orientation for the tensile tests.
3 Fig.2: One side injected plate to cut tensile coupons Tensile tests are performed at different strain rate (0.001/sec to 100/sec). The results will be used to create two different microstructural material models:  Isotropic nonlinear elastoviscoplastic for the thermoplastic matrix  Isotropic linear elastic for the glass fibers The identification of the material parameters is done by reverse engineering to fit the tests results with a homogenization method (Digimat or with a 3D representative volume element). Once the two micromaterial models are created, some tensile simulations with different fiber orientation tensors will be performed to export anisotropic flow curves. The composite material will be discretized regarding fiber orientation from an isotropic material with an average fiber orientation between the principal directions until a highly orthotropic material with 100% of the fibers in the major principal direction. Fig.3: Flow curve export with average fiber orientation (50% of fibers in 0 and 90, left) and highly oriented fibers (100 % of the fibers in 0, right) The material fiber orientation discretization has been setup every 5% of the fiber orientation tensor which is also defined in the mapping tool to affect the same material properties regarding fiber orientation distribution between the principal directions. For shell elements with 5% of fiber orientation tensor discretization, the total number of *MAT_ANISOTROPIC_ELASTIC_PLASTIC will be eleven: a 11 = 0,50 a 12 = 0 a 13 = 0 a 11 = 0,55 a 12 = 0 a 13 = 0 a 11 = 0,60 a 12 = 0 a 13 = 0 a 21 = 0 a 22 = 0,50 a 23 = 0, a 21 = 0 a 22 = 0,45 a 23 = 0, a 21 = 0 a 22 = 0,40 a 23 = 0, a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0 a 11 = 0,65 a 12 = 0 a 13 = 0 a 11 = 0,70 a 12 = 0 a 13 = 0 a 11 = 0,75 a 12 = 0 a 13 = 0 a 21 = 0 a 22 = 0,35 a 23 = 0, a 21 = 0 a 22 = 0,30 a 23 = 0, a 21 = 0 a 22 = 0,25 a 23 = 0, a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0
4 a 11 = 0,80 a 12 = 0 a 13 = 0 a 11 = 0,85 a 12 = 0 a 13 = 0 a 11 = 0,90 a 12 = 0 a 13 = 0 a 21 = 0 a 22 = 0,20 a 23 = 0, a 21 = 0 a 22 = 0,15 a 23 = 0, a 21 = 0 a 22 = 0,10 a 23 = 0, a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0 a 11 = 0,95 a 12 = 0 a 13 = 0 a 11 = 1,00 a 12 = 0 a 13 = 0 a 21 = 0 a 22 = 0,05 a 23 = 0, a 21 = 0 a 22 = 0,00 a 23 = 0 a 31 = 0 a 32 = 0 a 33 = 0 a 31 = 0 a 32 = 0 a 33 = 0 4 LSDyna anisotropic elastoviscoplastic material model *MAT_ANISOTROPIC_ELASTIC_PLASTIC Dynamore developed some new features of the *MAT_ANISOTROPIC_ELASTIC_PLASTIC to integrate strain rate sensitivity for anisotropic plasticity with VP=1 option (LSDyna Dev 88716). The *MAT_ANISOTROPIC_ELASTIC_PLASTIC (*MAT_157) is a combination of the *MAT_ANISOTROPIC_ELASTIC (*MAT_002_ANIS) which is the anisotropic stiffness matrix with the *MAT_ANISOTROPIC_VISCOPLASTIC (*MAT_103_P) which is isotropic linear elastic and anisotropic nonlinear viscoplastic. So the *MAT_ANISOTROPIC_ELASTIC_PLASTIC (*MAT_157) is:  Anisotropic linear elastic  Anisotropic stiffness matrix (36 parameters reduced to 21 with symetry) : σ ij = C ijkl ε kl  σ 11 σ 22 σ 33 σ 12 = σ 23 σ 31 C 11 C 12 C 13 C 21 C 22 C 23 C 31 C 32 C 33 C 41 C 42 C 43 C 51 C 52 C 53 C 61 C 62 C 63 C 14 C 15 C 16 C 24 C 25 C 26 C 34 C 35 C 36 C 44 C 45 C 46 C 54 C 55 C 56 C 64 C 65 C 66 ε 11 ε 22 ε 33 ε 12 ε 23 ε 31  For Orthotropic materials (fibers reinforced plastics), the stiffness matrix is reduced to 9 parameters :   σ 11 σ 22 σ 33 σ 12 = σ 23 σ 31 σ 11 σ 22 σ 33 σ 12 = σ 23 σ 31 C 11 C 12 C 13 C 12 C 22 C 23 C 13 C 23 C 33 1 υ 23υ 32 E 22 E 33 Δ υ 12 +υ 13 υ 32 E 11 E 33 Δ υ 13 +υ 12 υ 23 E 11 E 22 Δ C C C 66 υ 21 +υ 31 υ 23 E 22 E 33 Δ 1 υ 13 υ 31 E 11 E 33 Δ υ 23 +υ 13 υ 21 E 11 E 22 Δ υ 31 +υ 21 υ 32 E 22 E 33 Δ υ 32 +υ 12 υ 31 E 11 E 33 Δ 1 υ 12 υ 21 E 11 E 22 Δ  Δ = 1 υ 12υ 21 υ 23 υ 32 υ 31 υ 13 2υ 12 υ 23 υ 31 E 11 E 22 E 33  υ 21 = υ 12 ; υ 31 = υ 13 ; υ 32 = υ 23 E 22 E 11 E 33 E 11 E 33 E 22 ε 11 ε 22 ε 33 ε 12 ε 23 ε 31 2G G G 31 ε 11 ε 22 ε 33 ε 12 ε 23 ε 31  Anisotropic nonlinear viscoplastic  Tabulated flow curves (True Stress versus Effective Plastic Strain) versus strain rate  Anisotropic Hill s parameters R00, R45, R90 (for shell) that will modify the plasticity response for 0, 45, 90 angles This material model is able to simulate anisotropy induced by the short fiber orientation inside the thermoplastic.
5 The final FEA model integrates the fiber orientation by orienting elements and shell thickness integration points and the anisotropy linked to the fiber repartition between the different fiber principal directions. The numerical stability is similar to a *MAT_PIECEWISE_LINEAR_PLASTICITY (*MAT_024) with an excellent computation time, 100% under LSDyna without any external software coupling. This simulation method is applicable for an industrial / project approach and already deployed at Faurecia. But some limitations regarding the real material behavior are still done:  The material is not viscoelastic.  There is no triaxiality dependency for the flow curves. 5 Failure modeling by element erosion: *MAT_ADD_EROSION The rupture of the fiber reinforced plastic will depend on the following parameters  Fiber orientation  Strain rate  Triaxiality The material is brittle so the damage function by softening is not used. *MAT_ANISOTROPIC_ELASTIC_PLASTIC has no failure criteria included, so *MAT_ADD_EROSION is used to define failure criteria by element erosion. Two different isotropic failure conditions are applied to represent anisotropic failure:  Maximum Stress Von Mises for Longitudinal (0 axis) failure versus Strain rate (SIGVM with LCID)  Maximum Anisotropic Effective Plastic Strain for transversal (90 axis) failure versus Triaxiality versus Strain rate (IDAM=1, GISSMO with dmgtyp=81) As the stiffness is much higher for the longitudinal axis, the maximum stress values will not be reached by the transverse axis, and the maximum strain values for the transverse axis will not be reached in the longitudinal axis because the stress at failure will occur before. If one of the two failure conditions is reached (ncs=1), the thickness integration point fails. If more than 80% of the thickness integration points fail (Faurecia setting), then the element is suppressed. The *MAT_ADD_EROSION fiber orientation decomposition will follow the same *MAT_ANISOTROPIC_ELASTIC_PLASTIC decomposition. So if 11 *MAT_157 are created, 11 correspondent *MAT_ADD_EROSION will be added. The maximum stress and strain values are measured by testing and/or composite homogenization simulations.
6 Fig.4: Stress vs Strain Uniaxial tension strain rate dependency with failure (80% of the fibers in 0 and 20% in 90 principal direction) 6 Correlation on beams Static and dynamic three points bending tests have been performed on plastic beams with omega profile and cross ribs inside with different injections gates to have tests results versus injection process configurations. The beams have been molded with one or three gates injection configuration with a different fiber orientation tensor in the middle / impact area. Fig.5: One injection gate (left) / Three injection gates (right) beam fiber orientation results 6.1 LSDyna anisotropic beam model The mapping process has been applied to orient elements and anisotropic material (*MAT_157) for each molding configurations. The beam FEA model contains: *ELEMENT_SHELL_BETA *PART_COMPOSITE
7  12 layers oriented according the rheology simulation major principal fiber orientation output  Elform 16 full integration  11 *MAT_ANISOTROPIC_ELASTIC_PLASTIC with 11 *MAT_ADD_EROSION which corresponds to the composite homogenized material discretization with failure erosion criteria regarding fiber ratio between principals fiber directions Fig.6: LSDyna Dynamic three points bending Faurecia Matcar beam anisotropic elastoviscoplastic model 6.2 Static three points bending The beam profile is placed in a horizontal position, and the impactor has a fixed velocity. Material strain rate sensitivity is removed. The contact force versus the impactor displacement is measured. Fig.7: Static three points bending Simulations / Tests results for one and three injection gates (PA6 I GF35 23 C dry) Simulation and tests results show different results between injection configurations. The beam stiffness is increased for the one injection gate configuration due to a better fiber orientation in the beam length. Simulations and tests are closed for the stiffness and the load at rupture. A difference of 4 mm versus test result is observed for the maximum displacement with one injection gate model.
8 6.3 Dynamic three points bending The beam profile is placed in vertical position, the drop impactor has an initial veloticy of 2,37 m/s with a weight of 55 kg (155 J). Impactor deceleration is measured. Fig.8: Dynamic three points bending superposition Test / Simulation 1 injection gate (left), 3 injection gates (right) Simulations and tests results show different results for the one and three injection gates configurations with the same effects. Acceleration values are higher with the three injection gates beam due to higher strain at break in the beam impact area produced by the diffuse fiber orientation. Simulation results are slightly shifted in the time scale with a maximum acceleration peak 2g lower than tests results. Fig.9: Dynamic three points bending simulations / tests results Force versus Displacement Viscoelasticity of the material is not modelized and the beam is progressively damaged by cracks propagations which are mesh dependent and more difficult to simulate.
9 7 Conclusion Integration of anisotropic injection molding process effect of the short fiber orientation inside thermoplastics materials has been modelized with LSDyna *MAT_ANISOTROPIC_ELASTIC_PLASTIC. The definition of a mapping tool between process simulation and structural LSDyna simulation will define material discretization versus fiber orientation tensor and orient each element and each thickness integration points. Specific anisotropic material characterizations on injected plates with micro / macro scales homogenizations are required to define material decomposition regarding fiber orientation tensor. *MAT_157 is an anisotropic nonlinear elastoviscoplastic integrating principals anisotropic characteristics of the short fibers reinforced plastics for quasistatic and crash structural simulations. The correlations on Faurecia beams are demonstrating a good level of correlation with the influence of the injection process. This LSDyna anisotropic nonlinear elastoviscoplastic method improves simulation accuracy with a small computation time increase versus an isotropic method and a very good numerical stability without licence added cost.
14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationRecent Developments in Damage and Failure Modeling with LSDYNA
Recent evelopments in amage and Failure Modeling with LSYNA r. André Haufe ynamore GmbH Frieder Neukamm, r. Markus Feucht aimler AG Paul ubois Consultant r. Thomas Borvall ERAB 1 Technological challenges
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More information*MAT_PAPER  a new orthotropic elastoplastic model for paper materials
*MAT_PAPER  a new orthotropic elastoplastic model for paper materials Jesper Karlsson, Dynamore Nordic Mikael Schill, Dynamore Nordic Johan Tryding, Tetra Pak *MAT_PAPER (*MAT_274) A new orthotropic elastoplastic
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationLecture #10: Anisotropic plasticity Crashworthiness Basics of shell elements
Lecture #10: 1510735: Dynamic behavior of materials and structures Anisotropic plasticity Crashworthiness Basics of shell elements by Dirk Mohr ETH Zurich, Department of Mechanical and Process Engineering,
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationAnisotropic plasticity, anisotropic failure and their application to the simulation of aluminium extrusions under crash loads
Anisotropic plasticity, anisotropic failure and their application to the simulation of aluminium extrusions under crash loads Paul Du Bois, Consulting engineer Oasys LSDYNA Users Meeting 28th January
More informationDon Robbins, Andrew Morrison, Rick Dalgarno Autodesk, Inc., Laramie, Wyoming. Abstract
PROGRESSIVE FAILURE SIMULATION OF ASMANUFACTURED SHORT FIBER FILLED INJECTION MOLDED PARTS: VALIDATION FOR COMPLEX GEOMETRIES AND COMBINED LOAD CONDITIONS Don Robbins, Andrew Morrison, Rick Dalgarno Autodesk,
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationSOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS
Mechanical Testing and Diagnosis ISSN 2247 9635, 2012 (II), Volume 3, 7985 SOME RESEARCH ON FINITE ELEMENT ANALYSIS OF COMPOSITE MATERIALS Valeriu DULGHERU, Viorel BOSTAN, Marin GUŢU Technical University
More informationModelling the Rheology of SemiConcentrated Polymeric Composites
THALES Project No 1188 Modelling the Rheology of SemiConcentrated Polymeric Composites Research Team Evan Mitsoulis (PI), Professor, NTUA, Greece Costas Papoulias (Research Student), NTUA, Greece Souzanna
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More information3D Compression Molding
Autodesk Simulation Moldflow Insight 2014 3D Compression Molding Executive summary In this work, the simulation results from a program developed for the threedimensional analysis of compression molding
More informationPressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials
Pressure Vessels Stresses Under Combined Loads Yield Criteria for Ductile Materials and Fracture Criteria for Brittle Materials Pressure Vessels: In the previous lectures we have discussed elements subjected
More informationBone Tissue Mechanics
Bone Tissue Mechanics João Folgado Paulo R. Fernandes Instituto Superior Técnico, 2016 PART 1 and 2 Introduction The objective of this course is to study basic concepts on hard tissue mechanics. Hard tissue
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationME 582 Advanced Materials Science. Chapter 2 Macromechanical Analysis of a Lamina (Part 2)
ME 582 Advanced Materials Science Chapter 2 Macromechanical Analysis of a Lamina (Part 2) Laboratory for Composite Materials Research Department of Mechanical Engineering University of South Alabama, Mobile,
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationImpact and Fracture Mechanics Assessment of a Fused Silica Window
Arnold AFB Wind Tunnel Impact and Fracture Mechanics Analysis Rev0 1 of 41 Impact and Fracture Mechanics Assessment of a Fused Silica Window Objective: Determine the survival probability of a fused silica
More informationFinite element analysis of diagonal tension failure in RC beams
Finite element analysis of diagonal tension failure in RC beams T. Hasegawa Institute of Technology, Shimizu Corporation, Tokyo, Japan ABSTRACT: Finite element analysis of diagonal tension failure in a
More informationUnified Constitutive Model for Engineering Pavement Materials and Computer Applications. University of Illinois 12 February 2009
Unified Constitutive Model for Engineering Pavement Materials and Computer Applications Chandrakant S. Desai Kent Distinguished i Lecture University of Illinois 12 February 2009 Participation in Pavements.
More informationBending of Simply Supported Isotropic and Composite Laminate Plates
Bending of Simply Supported Isotropic and Composite Laminate Plates Ernesto GutierrezMiravete 1 Isotropic Plates Consider simply a supported rectangular plate of isotropic material (length a, width b,
More informationGeology 229 Engineering Geology. Lecture 5. Engineering Properties of Rocks (West, Ch. 6)
Geology 229 Engineering Geology Lecture 5 Engineering Properties of Rocks (West, Ch. 6) Common mechanic properties: Density; Elastic properties:  elastic modulii Outline of this Lecture 1. Uniaxial rock
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More information3. Overview of MSC/NASTRAN
3. Overview of MSC/NASTRAN MSC/NASTRAN is a general purpose finite element analysis program used in the field of static, dynamic, nonlinear, thermal, and optimization and is a FORTRAN program containing
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More information9 Strength Theories of Lamina
9 trength Theories of Lamina 9 TRENGTH O ORTHOTROPIC LAMINA or isotropic materials the simplest method to predict failure is to compare the applied stresses to the strengths or some other allowable stresses.
More informationINTRODUCTION TO THE EXPLICIT FINITE ELEMENT METHOD FOR NONLINEAR TRANSIENT DYNAMICS
INTRODUCTION TO THE EXPLICIT FINITE ELEMENT METHOD FOR NONLINEAR TRANSIENT DYNAMICS SHEN R. WU and LEI GU WILEY A JOHN WILEY & SONS, INC., PUBLICATION ! PREFACE xv PARTI FUNDAMENTALS 1 1 INTRODUCTION 3
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationDevelopment, implementation and Validation of 3D Failure Model for Aluminium 2024 for High Speed Impact Applications
Development, implementation and Validation of D Failure Model for Aluminium 2024 for High Speed Impact Applications Paul Du Bois, Murat Buyuk, Jeanne He, Steve Kan NCACGWU th International LSDYNA Users
More informationTHERMOMECHANICAL BEHAVIOUR OF SHORT GLASS FIBRE REINFORCED POLYAMIDE
THERMOMECHANICAL BEHAVIOUR OF SHORT GLASS FIBRE REINFORCED POLYAMIDE A. Ayadi a,b, F. Roger a*, H. Nouri a, H. Maitournam c and I. Raoult d a Mines Douai, Department of Polymers and Composites Technology
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationMODELING OF CONCRETE MATERIALS AND STRUCTURES. Kaspar Willam. Isotropic Elastic Models: Invariant vs Principal Formulations
MODELING OF CONCRETE MATERIALS AND STRUCTURES Kaspar Willam University of Colorado at Boulder Class Meeting #2: Nonlinear Elastic Models Isotropic Elastic Models: Invariant vs Principal Formulations Elastic
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More information3dimensional joint torque calculation of compression sportswear using 3DCG human model
3dimensional joint torque calculation of compression sportswear using 3DCG human model Akihiro Matsuda, University of Tsukuba Hirokazu Tanaka, University of Tsukuba Hitoshi Aoki, University of Tsukuba
More informationBACKGROUNDS. Two Models of Deformable Body. Distinct Element Method (DEM)
BACKGROUNDS Two Models of Deformable Body continuum rigidbody spring deformation expressed in terms of field variables assembly of rigidbodies connected by spring Distinct Element Method (DEM) simple
More informationNONLINEAR STATIC SIMULATION OF AUTOMOTIVE BUMPER OF A PASSENGER CAR IN LOW SPEED IMPACT CRASH SIMULATION
NONLINEAR STATIC SIMULATION OF AUTOMOTIVE BUMPER OF A PASSENGER CAR IN LOW SPEED IMPACT CRASH SIMULATION Rajshekhar A Kharde 1, S. F. Patil 2 1 M.Tech Student, KLE Dr. M.S Sheshgiri College of Engg & Tech,
More informationPredicting Fatigue Life with ANSYS Workbench
Predicting Fatigue Life with ANSYS Workbench How To Design Products That Meet Their Intended Design Life Requirements Raymond L. Browell, P. E. Product Manager New Technologies ANSYS, Inc. Al Hancq Development
More informationEnhancement of Spot Weld Modeling using MAT 100 DAI
7. LSDYNA Anwenderforum, Bamberg 2008 Crash II  Verbindungstechnik, Versagen Enhancement of Spot Weld Modeling using MAT 100 DAI Falko Seeger a, Markus Feucht a, George Dumitru b, Tobias Graf b a Daimler
More informationEvaluation of Material Models to Predict Material Failure in LSDYNA
Department of Construction Sciences Solid Mechanics ISRN LUTFD2/TFHF16/5209SE(155) Evaluation of Material Models to Predict Material Failure in LSDYNA Master s Dissertation by Hjalmar Sandberg Oscar
More informationNumerical simulation the bottom structures. grounding test by LSDYNA
5 th European LSDYNA Users Conference Methods and Techniques (3) Numerical simulation the bottom structures grounding test by LSDYNA Ainian Zhang Graduate School of Frontier Sciences, The University
More informationThe Design of Polyurethane Parts: Using Closed Solutions and Finite Element Analysis to Obtain Optimal Results
The Design of Polyurethane Parts: Using Closed Solutions and Finite Element Analysis to Obtain Optimal Results By: Richard Palinkas George Nybakken Ian Laskowitz Chemtura Corporation Overview How does
More informationFigure 1 Lifting Lug Geometry with Weld
Should you Perform Nonlinear Stress Analysis? Many of our clients inquire whether nonlinearity should be considered in their analyses. The answer to that question is not simple. Sometimes, as in certain
More informationChapter 2  Macromechanical Analysis of a Lamina. Exercise Set. 2.1 The number of independent elastic constants in three dimensions are: 2.
Chapter  Macromechanical Analysis of a Lamina Exercise Set. The number of independent elastic constants in three dimensions are: Anisotropic Monoclinic 3 Orthotropic 9 Transversely Orthotropic 5 Isotropic.
More informationNonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. F Talence, France Le Cheylard, France
20 th International Conference on Composite Materials Copenhagen, 1924th July 2015 Nonconventional Glass fiber NCF composites with thermoset and thermoplastic matrices. Thierry Lorriot 1, Jalal El Yagoubi
More informationAim of the study Experimental determination of mechanical parameters Local buckling (wrinkling) Failure maps Optimization of sandwich panels
METNET Workshop October 1112, 2009, Poznań, Poland Experimental and numerical analysis of sandwich metal panels Zbigniew Pozorski, Monika ChudaKowalska, Robert Studziński, Andrzej Garstecki Poznan University
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationExample3. Title. Description. Cylindrical Hole in an Infinite MohrCoulomb Medium
Example3 Title Cylindrical Hole in an Infinite MohrCoulomb Medium Description The problem concerns the determination of stresses and displacements for the case of a cylindrical hole in an infinite elastoplastic
More informationBuckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate
Buckling Behavior of 3D Randomly Oriented CNT Reinforced Nanocomposite Plate Outline Introduction Representative Volume Element (RVE) Periodic Boundary Conditions on RVE Homogenization Method Analytical
More informationEFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING
Journal of MECHANICAL ENGINEERING Strojnícky časopis, VOL 67 (217), NO 1, 522 EFFECT OF LAMINATION ANGLE AND THICKNESS ON ANALYSIS OF COMPOSITE PLATE UNDER THERMO MECHANICAL LOADING Arnab Choudhury 1,
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationA PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL
A PAPER ON DESIGN AND ANALYSIS OF PRESSURE VESSEL P.Palanivelu 1, R.Siva Prasad 2, 1 PG Scholar, Department of Mechanical Engineering, Gojan School of Business and Technology, Redhills, Chennai, India.
More informationAcetone Polishing of ABS Test Results
Acetone Polishing of ABS Test Results Date: Objective: June 16, 16 Determine Effect of Acetone on Mechanical Strength of 3D Printed Objects in Different Print Orientaions. Equipment: TestrBot, PrintrBot,
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationVALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 )
VALIDATION of CoDA SOFTWARE for COMPOSITES SYNTHESIS AND PRELIMINARY DESIGN (or GETTING COMPOSITES USED  PART 2 ) Graham D Sims and William R Broughton Composites Design Data and Methods, Centre for Materials
More informationFINITE ELEMENT ANALYSIS OF A LAYERED COMPOSITE CYLINDER USING THE CONNECTION BETWEEN THE MACRO AND MICROSTRUCTURE
FINITE ELEMENT ANALYI OF A LAYERED COMPOITE CYLINDER UING THE CONNECTION BETWEEN THE MACRO AND MICROTRUCTURE A. zekrényes Research Assistant, Department of Applied Mechanics, Budapest University of Technology
More informationThis guide is made for nonexperienced FEA users. It provides basic knowledge needed to start your fatigue calculations quickly.
Quick Fatigue Analysis Guide This guide is made for nonexperienced FEA users. It provides basic knowledge needed to start your fatigue calculations quickly. Experienced FEA analysts can also use this
More informationInternational Journal of Advanced Engineering Technology EISSN
Research Article INTEGRATED FORCE METHOD FOR FIBER REINFORCED COMPOSITE PLATE BENDING PROBLEMS Doiphode G. S., Patodi S. C.* Address for Correspondence Assistant Professor, Applied Mechanics Department,
More informationEXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES
EXPERIMENTAL AND NUMERICAL STUDY OF THE ENERGY ABSORPTION CAPACITY OF PULTRUDED COMPOSITE TUBES D. Kakogiannis 1, D. Van Hemelrijck 1, J. Wastiels 1, S. Palanivelu 2, W. Van Paepegem 2, K. De Wolf 3, J.
More informationSemiloof Curved Thin Shell Elements
Semiloof Curved Thin Shell Elements General Element Name Y,v,θy X,u,θx Z,w,θz Element Group Element Subgroup Element Description Number Of Nodes Freedoms Node Coordinates TSL 1 2 Semiloof 3 QSL8 7 8 1
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationFinite Element Analysis of Wood and Composite Structured Hockey sticks
Finite Element Analysis of Wood and Composite Structured Hockey sticks 605 Finite Element Analysis Professor Ian Grosse May 15, 2003 By: Michael O Brien Project Statement The direction of this project
More informationAutodesk Moldflow Insight AMI Fiber Orientation Analysis
Autodesk Moldflow Insight 2012 AMI Fiber Orientation Analysis Revision 1, 22 March 2012. This document contains Autodesk and thirdparty software license agreements/notices and/or additional terms and
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationFINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND
FINITE ELEMENT MODELING OF DELAMINATION DAMAGE IN CARBON FIBER LAMINATES SUBJECT TO LOWVELOCITY IMPACT AND COMPARISON WITH EXPERIMENTAL IMPACT TESTS USING NONDESTRUCTIVE VIBROTHERMOGRAPHY EVALUATION A
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationEFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS
EFFECT OF SHEAR REINFORCEMENT ON FAILURE MODE OF RC BRIDGE PIERS SUBJECTED TO STRONG EARTHQUAKE MOTIONS Atsuhiko MACHIDA And Khairy H ABDELKAREEM SUMMARY Nonlinear D FEM was utilized to carry out inelastic
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationChapter 5 Elastic Strain, Deflection, and Stability 1. Elastic StressStrain Relationship
Chapter 5 Elastic Strain, Deflection, and Stability Elastic StressStrain Relationship A stress in the xdirection causes a strain in the xdirection by σ x also causes a strain in the ydirection & zdirection
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More information3D and Planar Constitutive Relations
3D and Planar Constitutive Relations A School on Mechanics of Fibre Reinforced Polymer Composites Knowledge Incubation for TEQIP Indian Institute of Technology Kanpur PM Mohite Department of Aerospace
More informationMATERIAL ELASTIC ANISOTROPIC command
MATERIAL ELASTIC ANISOTROPIC command.. Synopsis The MATERIAL ELASTIC ANISOTROPIC command is used to specify the parameters associated with an anisotropic linear elastic material idealization. Syntax The
More informationUnderstand basic stressstrain response of engineering materials.
Module 3 Constitutive quations Learning Objectives Understand basic stressstrain response of engineering materials. Quantify the linear elastic stressstrain response in terms of tensorial quantities
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationENGN 2290: Plasticity Computational plasticity in Abaqus
ENGN 229: Plasticity Computational plasticity in Abaqus The purpose of these exercises is to build a familiarity with using usermaterial subroutines (UMATs) in Abaqus/Standard. Abaqus/Standard is a finiteelement
More informationEVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS EVALUATION OF DAMAGE DEVELOPMENT FOR NCF COMPOSITES WITH A CIRCULAR HOLE BASED ON MULTISCALE ANALYSIS T. Kurashiki 1 *, Y. Matsushima 1, Y. Nakayasu
More informationDetermination of the Shear Buckling Load of a Large Polymer Composite ISection Using Strain and Displacement Sensors
Sensors 2012, 12, 1602416036; doi:10.3390/s121216024 Article OPEN ACCESS sensors ISSN 14248220 www.mdpi.com/journal/sensors Determination of the Shear Buckling Load of a Large Polymer Composite ISection
More informationModeling the bond of GFRP and concrete based on a damage evolution approach
Modeling the ond of GFRP and concrete ased on a damage evolution approach Mohammadali Rezazadeh 1, Valter Carvelli 2, and Ana Veljkovic 3 1 Dep. Architecture, Built environment and Construction engineering,
More informationBasics of Finite Element Analysis. Strength of Materials, Solid Mechanics
Basics of Finite Element Analysis Strength of Materials, Solid Mechanics 1 Outline of Presentation Basic concepts in mathematics Analogies and applications Approximations to Actual Applications Improvisation
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationStatic & Dynamic. Analysis of Structures. Edward L.Wilson. University of California, Berkeley. Fourth Edition. Professor Emeritus of Civil Engineering
Static & Dynamic Analysis of Structures A Physical Approach With Emphasis on Earthquake Engineering Edward LWilson Professor Emeritus of Civil Engineering University of California, Berkeley Fourth Edition
More informationExperimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 pebbles
Experimental and theoretical characterization of Li 2 TiO 3 and Li 4 SiO 4 s D. Aquaro 1 N. Zaccari ABSTRACT Dipartimento di Ingegneria Meccanica Nucleare e della Produzione University of Pisa (Italy)
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationPlane Strain Test for Metal Sheet Characterization
Plane Strain Test for Metal Sheet Characterization Paulo Flores 1, Felix Bonnet 2 and AnneMarie Habraken 3 1 DIM, University of Concepción, Edmundo Larenas 270, Concepción, Chile 2 ENS  Cachan, Avenue
More information**********************************************************************
Department of Civil and Environmental Engineering School of Mining and Petroleum Engineering 333 Markin/CNRL Natural Resources Engineering Facility www.engineering.ualberta.ca/civil Tel: 780.492.4235
More informationScienceDirect. Unit cell model of woven fabric textile composite for multiscale analysis. Anurag Dixit a *,Harlal Singh Mali b, R.K.
Available online at www.sciencedirect.com ScienceDirect Procedia Engineering 68 ( 2013 ) 352 358 The Malaysian International Tribology Conference 2013 (MITC2013) Unit cell model of woven fabric textile
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More information